Hindawi Publishing Corporation International Journal of Dentistry Volume 2016, Article ID 7094056, 6 pages http://dx.doi.org/10.1155/2016/7094056
Research Article The Reinforcement Effect of Nano-Zirconia on the Transverse Strength of Repaired Acrylic Denture Base Mohammed Gad,1 Aws S. ArRejaie,1 Mohamed Saber Abdel-Halim,1 and Ahmed Rahoma2,3 1
Department of Substitutive Dental Sciences, College of Dentistry, University of Dammam, P.O. Box 1982, Dammam 31411, Saudi Arabia 2 Department of Biomaterial Dental Sciences, College of Dentistry, University of Dammam, P.O. Box 1982, Dammam 31411, Saudi Arabia 3 Department of Dental Materials, College of Dentistry, Al-Azhar University, P.O. Box 11117, Assiut, Egypt Correspondence should be addressed to Mohammed Gad; [email protected]
Received 18 March 2016; Accepted 9 May 2016 Academic Editor: Jamil A. Shibli Copyright © 2016 Mohammed Gad et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited. Objective. The aim of this study was to evaluate the effect of incorporation of glass fiber, zirconia, and nano-zirconia on the transverse strength of repaired denture base. Materials and Methods. Eighty specimens of heat polymerized acrylic resin were prepared and randomly divided into eight groups (𝑛 = 10): one intact group (control) and seven repaired groups. One group was repaired with autopolymerized resin while the other six groups were repaired using autopolymerized resin reinforced with 2 wt% or 5 wt% glass fiber, zirconia, or nano-zirconia particles. A three-point bending test was used to measure the transverse strength. The results were analyzed using SPSS and repeated measure ANOVA and post hoc least significance (LSD) test (𝑃 ≤ 0.05). Results. Among repaired groups it was found that autopolymerized resin reinforced with 2 or 5 wt% nano-zirconia showed the highest transverse strength (𝑃 ≤ 0.05). Repairs with autopolymerized acrylic resin reinforced with 5 wt% zirconia showed the lowest transverse strength value. There was no significant difference between the groups repaired with repair resin without reinforcement, 2 wt% zirconia, and glass fiber reinforced resin. Conclusion. Reinforcing of repair material with nano-zirconia may significantly improve the transverse strength of some fractured denture base polymers.
1. Introduction Denture fracture is a common problem in prosthodontic practice that troubles both patients and prosthodontists. Inordinate masticatory forces or denture deformation during use can result in bending forces that contribute to fatigue of the material and subsequent fracture . A new denture construction increases the cost and is time consuming, so denture repair is preferred . Satisfactory repair should be easy and rapid and match the original color of the denture base while maintaining the dimensional accuracy . Denture repair depends on many variables including material type, material reinforcement, surface design, and surface treatment . Several materials have been used to repair fractured denture bases, including autopolymerized, visible light polymerized, heat polymerized, or microwave polymerized acrylic resin [4, 5]. Most (86%) of denture base repairs are made with
autopolymerized acrylic resin  because it is easy to manipulate and fast and can be used chair-side . Unfortunately, its strength has been shown to range from 18 to 81% of intact heat polymerized denture resin [3, 8]. Many attempts have been made to overcome this shortcoming via using reinforced repair material and/or modification of repair surface design and treatment. Hanna et al. investigated the effect of 45∘ bevel of the repair surface on the transverse strength of the repaired denture base and found that higher values were obtained . Beveling of the repair surface changed the fracture type from weak adhesive to strong cohesive fracture . It is appropriate to treat the repair surface with repair monomer as it modifies the surface structure and increases its bond to repair material [11–13]. Glass fiber is one of the most common reinforcement materials and many investigations of its effect on repaired
International Journal of Dentistry Table 1: Tested groups and coding according to repair material reinforcement.
Group code HC AP 2GF 5GF 2ZR 5ZR 2NZR 5NZR
denture base have been performed. Addition of glass fiber to repair material improves the strength of a denture base repair and may decrease the occurrence of future fracture [3, 14, 15]. This may be attributed to the fact that glass fiber has a high resilience which allows the stresses to be received by them without deformation . Zirconia (ZrO2 ) is a metal oxide and may be used as a reinforcement material to improve the transverse strength of denture base resin [17, 18]. Reinforcement of acrylic denture base with zirconia significantly increases its transverse strength . Recently, nanotechnology invaded the prosthodontic field for medical and material enhancement purposes. The properties of the reinforced resin by nanoparticles depend on the size, shape, type, and concentration of the added particles . Additions of nano-zirconia to polymethylmethacrylate (PMMA) denture base have been reported to increase the transverse strength due to its small size and homogenous distribution . The disadvantage of commonly used repair materials is that they have poor strength. The current research in the field of dental materials is focused on finding the appropriate repair material with adequate strength and prolonged shelf life. Till date, the effect of nano-ZrO2 on repair strength has not been investigated. Therefore, this study was conducted to evaluate the reinforcement effect of different concentrations of glass fiber, zirconia, and nano-zirconia on the transverse strength of a repaired denture base. The null hypothesis was that the addition of different concentrations of zirconia or nano-zirconia will not improve the transverse strength of repaired denture base.
2. Materials and Methods In accordance with ANSI/ADA specification number 12, eighty rectangular specimens of heat polymerized acrylic resin with dimensions (65 × 10 × 2.5 mm ± 0.1) were prepared using customized molds . Molds were waxed up (Cavex Set Up Wax, Cavex, Netherlands) and then wax patterns were invested in type III dental stone (GC Fujirock EP, Belgium) within a flask (61B Two Flask Compress, Handler Manufacturing, USA) and then dewaxed to create the mold space. According to the manufacturer’s instructions, heat polymerized acrylic resin (Major Base 20, Major Prodotti Dentari SPA, Italy) was mixed and packed in the dough stage into the mold cavity and trial closure was done and then flask was closed and kept under bench press for 30 min. Flask with
Repair material Intact heat polymerized specimens (control) Autopolymerized acrylic resin Autopolymerized acrylic resin reinforced with 2 wt% glass fiber Autopolymerized acrylic resin reinforced with 5 wt% glass fiber Autopolymerized acrylic resin reinforced with 2 wt% zirconia Autopolymerized acrylic resin reinforced with 5 wt% zirconia Autopolymerized acrylic resin reinforced with 2 wt% nano-zirconia Autopolymerized acrylic resin reinforced with 5 wt% nano-zirconia
acrylic resin specimens was processed for 8 hours in water bath at 74∘ C and then temperature was increased to 100∘ C for 1 hour into thermal curing unit (KaVo Elektrotechnisches Werk GmbH, D-88299, Germany). After curing, the flasks were bench cooled to room temperature prior to deflasking. The excess resin of deflasked specimens was removed with a tungsten carbide bur (HM251 FX 040 HP, Meisinger, USA), polished with acrylic polisher (HM251FX-060, Meisinger, USA), and then stored in distilled water at 37∘ C for 48 hours. All specimens were randomly divided into eight groups: one intact and seven repaired groups (Table 1). To create 3 mm repair gap, repair specimens were placed into the mold and numbered on both ends for reassembling. Mark was drawn at the specimen center and then at 1.5 mm distance from this mark two lines were drawn on both sides and perpendicular to the long edge of specimen. These two lines were extended on the surfaces of the mold as a guide for all specimens. At these lines the specimens were cut with low speed diamond disc (DeguDent, GmbH, REF 59903107, Dentsply, Germany) under profuse irrigation. Standardized 45∘ bevel joint was prepared by measuring a 2.5 mm and drawing a line parallel to the prepared edge. In the same manner, the mold sides were cut at the center measuring 8 mm from the upper surface and 3 mm from the lower surface preserving the mold base intact. Specimens were placed in the mold and cut in bevel direction by diamond disc guided by lines and mold surfaces to create a repair gap of 3 mm × 10 mm × 2.5 mm with a 45∘ bevel joint. Glass fiber (E-glass; length = 3 mm, Shanghai Richem International Co., Ltd., China), zirconia (99.5%, 5 um, 1314-23-4, Shanghai Richem International Co., Ltd., China), and nano-zirconia powder (99.9%,